Preparation of 1,4-bis(4-methylstyryl)benzene nanocrystals by a wet process and evaluation of their optical properties
© Baba and Nishida; licensee Springer. 2014
Received: 25 October 2013
Accepted: 1 January 2014
Published: 13 January 2014
Single-crystal 1,4-bis(4-methylstyryl)benzene is a promising material for optoelectronic device applications. We demonstrate the preparation of 1,4-bis(4-methylstyryl)benzene nanocrystals by a wet process using a bottom-up reprecipitation technique. Scanning electron microscopy revealed the morphology of the nanocrystals to be sphere-like with an average particle size of about 60 nm. An aqueous dispersion of the nanocrystals was monodisperse and stable with a ζ-potential of -41 mV. The peak wavelengths of the absorption and emission spectra of the nanocrystal dispersion were blue and red shifted, respectively, compared with those of tetrahydrofuran solution. Powder X-ray diffraction analysis confirmed the crystallinity of the nanocrystals. The presented 1,4-bis(4-methylstyryl)benzene nanocrystals are expected to be a candidate for a new class of optoelectronic material.
KeywordsOrganic nanocrystal 1,4-bis(4-methylstyryl)benzene Water dispersion Bottom-up fabrication technique Wet process Optical properties
In contrast, we have investigated the preparation and evaluated the properties of nano-sized organic crystals, i.e., organic nanocrystals [8–11]. Organic nanocrystals show unique physicochemical properties different from those of the molecular and bulk crystal states [12–15]. Organic nanocrystals have been broadly used as optoelectronic materials as well as biomedical materials [16–22]. Recently, Fang et al. demonstrated the preparation of BSB-Me nanocrystals using a femtosecond laser-induced forward transfer method [23, 24]. The BSB-Me nanocrystals were directly deposited on a substrate to form a nanocrystal film, and their size and morphology were investigated as functions of applied laser fluence. The use of BSB-Me nanocrystals will be a promising approach for organic crystal device applications in the near future. However, according to Fang's report, the morphology of the prepared BSB-Me nanocrystals were multifarious, i.e., while most nanoparticles were cubic in geometry, others were tetrahedral shaped, truncated cubes, and truncated tetrahedra . To fabricate high-quality optical devices, such nanocrystals should ideally be homogenous in shape and in size because their optical properties are strongly affected by the crystal morphology. Additionally, there is a serious problem that the yields of nanoparticles prepared by laser ablation are smaller than those obtained by other nanoparticle synthesis methods because the nanocrystals are formed only in the small laser-irradiated spot . This is a weak point when considering mass production for device fabrication. Furthermore, the output power of laser ablation is not suitable for organic compounds because the high energy may degrade them [26, 27]. Wet processes using bottom-up techniques overcome these disadvantages. The solvent exchange method, known as the reprecipitation method, is especially suitable for preparing organic nanocrystals [18, 28]. Unlike laser ablation, no excess energy is necessary to form the organic nanocrystals, and bulk production is possible . Following a previously reported study, it is possible to prepare a nanocrystal-layered thin film for optical devices using the reprecipitation method . Instead of top-down laser ablation, the alternative approach of this bottom-up wet process is an attractive prospect for preparing BSB-Me nanocrystals.
The aim of this study is to demonstrate the preparation of BSB-Me nanocrystals having narrow size distribution with singular morphology by means of a bottom-up, wet process using the reprecipitation method. This method makes it possible to control the particle size and morphology of the nanocrystals. We prepared BSB-Me nanocrystal dispersions in water, and investigated the size, morphology, optical properties, and powder X-ray diffraction pattern of the nanocrystals.
BSB-Me (>98.0%) was purchased from Tokyo Chemical Industry Co., Ltd. (Tokyo, Japan) and used without further purification. Tetrahydrofuran (THF) (>99.5%) was purchased from Wako Pure Chemical Industries, Ltd. (Tokyo, Japan). Purified water (18.2 MΩ) was obtained from a Milli-Q A-10 (Millipore, Tokyo, Japan).
BSB-Me was dissolved in THF (2 mM) at 50°C, and 100 μl of the solution was injected into vigorously stirred (1,500 rpm) poor solvent water (10 ml at 24°C) using a microsyringe. As a result, the BSB-Me suddenly precipitated to form dispersed nanocrystals. Syringe filter (pore size 1.2 μm; Minisart®, Sartorius Stedim Biotech, NY, USA) was used to remove small degree of aggregates from the nanocrystal dispersion.
The particle size and morphology of the BSB-Me nanocrystals were evaluated using scanning electron microscopy (SEM; JSM-6510LA, JEOL, Tokyo, Japan). To prepare specimens for imaging, the nanocrystals were collected from the water dispersion using suction filtration with a membrane filter (0.05-μm pore size), followed by platinum sputter coating (JFC-1600, JEOL). The average particle size, size distribution, and ζ-potential of the nanocrystal dispersion were evaluated using an ELSZ-1000 zeta-potential and particle size analyzer (Otsuka Electronics Co., Ltd., Osaka, Japan). Ultraviolet-visible (UV-vis) absorption spectra and fluorescence spectra were measured using a V-550 UV/vis spectrophotometer (JASCO, Tokyo, Japan) and F-2500 fluorescence spectrophotometer (Hitachi, Tokyo, Japan), respectively.
Results and discussion
Quantum yield, integrated intensity, optical density, and refractive index of the BSB-Me
Quantum yield (Q),%
Integrated intensity (I)b
Optical density (OD) at λ = 324 nmc
Refractive index (n) at 20°C
BSB-Me dissolved in dichloromethane (1 μM)
95 ± 1a
BSB-Me nanocrystal water dispersion (2 μM)
9.2 ± 0.1
We demonstrated the preparation of a BSB-Me nanocrystal dispersion in water by the reprecipitation method, which is a bottom-up, wet process for preparing organic nanocrystals. SEM observations revealed that the nanocrystals had a sphere-like morphology. The average particle size was 60.9 nm, measured using an ELSZ-1000 zeta-potential and particle size analyzer. The nanocrystal dispersion was stable with a measured ζ-potential of -41.62 mV using ELSZ-1000. The blue shift and red shift of maximum peak wavelength were observed in absorption and emission spectra, respectively. This optical feature may have arisen from supramolecular interactions like those caused by the herringbone structure, i.e., H-aggregation, in the nanocrystals. The photoluminescence quantum yield of the BSB-Me nanocrystal water dispersion was estimated to be 9.2 ± 0.1%. Powder X-ray diffraction analysis confirmed the crystallinity of the BSB-Me nanocrystals. In future work, these BSB-Me nanocrystals will be applied to crystalline-based optoelectronic devices. Measuring amplified spontaneous emission and nonlinear optical properties of single nanocrystals will be a particularly interesting topic for the near future. We will also investigate and discuss elsewhere the nanocrystal size distribution using Scherrer's equation based on the data of XRD measurements. Further detailed optical properties such as an absolute photoluminescence quantum yield, fluorescence lifetime, and radiative decay rates of BSB-Me nanocrystals will be discussed elsewhere. Furthermore, fluorescent BSB-Me nanocrystals could be used in biological applications such as fluorescent bioimaging of cells and tissue similar to that in our previous work.
KB is an Endowed Chair Associate Professor at the Department of Visual Regenerative Medicine, Osaka University Graduate School of Medicine, Japan, and KN is a Professor and a medical doctor at the Department of Ophthalmology, Osaka University Graduate School of Medicine, Japan.
This study was partially supported by a Challenging Exploratory Research (no. 25560223) and Grant-in-Aid for Young Scientists (A) (no. 24680054) from the Japan Society for the Promotion of Science. We thank Dr. Yasunobu Wada for his technical support to the experiments.
- Yang J, Fang HH, Ding R, Lu SY, Zhang YL, Chen QD, Sun HB: High-quality large-size organic crystals prepared by improved physical vapor growth technique and their optical gain properties. J Phy Chem C 2011, 115: 9171–9175. 10.1021/jp110646nView ArticleGoogle Scholar
- Liu SH, Wang WCM, Briseno AL, Mannsfeld SCE, Bao ZN: Controlled deposition of crystalline organic semiconductors for field-effect-transistor applications. Adv Mater 2009, 21: 1217–1232. 10.1002/adma.200802202View ArticleGoogle Scholar
- Nakanotani H, Saito M, Nakamura H, Adachi C: Emission color tuning in ambipolar organic single-crystal field-effect transistors by dye-doping. Adv Funct Mater 2010, 20: 1610–1615. 10.1002/adfm.200902339View ArticleGoogle Scholar
- Sasaki F, Kobayashi S, Haraichi S, Fujiwara S, Bando K, Masumoto Y, Hotta S: Microdisk and microring lasers of thiophene-phenylene co-oligomers embedded in Si/SiO2 substrates. Adv Mater 2007, 19: 3653–3655. 10.1002/adma.200701008View ArticleGoogle Scholar
- Fang HH, Yang J, Ding R, Chen QD, Wang L, Xia H, Feng J, Ma YG, Sun HB: Polarization dependent two-photon properties in an organic crystal. Appl Phys Lett 2010, 97: 101101. 10.1063/1.3486683View ArticleGoogle Scholar
- Kabe R, Nakanotani H, Sakanoue T, Yahiro M, Adachi C: Effect of molecular morphology on amplified spontaneous emission of bis-styrylbenzene derivatives. Adv Mater 2009, 21: 4034–4038. 10.1002/adma.200803588View ArticleGoogle Scholar
- Nakanotani H, Adachi C: Organic light-emitting diodes containing multilayers of organic single crystals. Appl Phys Lett 2010, 96: 053301. 10.1063/1.3298558View ArticleGoogle Scholar
- Baba K, Kasai H, Nishida K, Nakanishi H: Poly( N -isopropylacrylamide)-based thermoresponsive behavior of fluorescent organic nanocrystals. Jpn J Appl Phys 2011, 50: 010202.View ArticleGoogle Scholar
- Baba K, Nishida K: Calpain inhibitor nanocrystals prepared using Nano Spray Dryer B-90. Nanoscale Res Lett 2012, 7: 436. 10.1186/1556-276X-7-436View ArticleGoogle Scholar
- Baba K, Nishida K: Steroid nanocrystals prepared using the Nano Spray Dryer B-90. Pharmaceutics 2013, 5: 107–114. 10.3390/pharmaceutics5010107View ArticleGoogle Scholar
- Baba K, Kasai H, Okada S, Oikawa H, Nakanishi H: Novel fabrication process of organic microcrystals using microwave-irradiation. Jpn J Appl Phys 2000, 39: L1256-L1258. 10.1143/JJAP.39.L1256View ArticleGoogle Scholar
- Katagi H, Kasai H, Okada S, Oikawa H, Komatsu K, Matsuda H, Liu ZF, Nakanishi H: Size control of polydiacetylene microcrystals. Jpn J Appl Phys 1996, 35: L1364-L1366. 10.1143/JJAP.35.L1364View ArticleGoogle Scholar
- Nakanishi H, Katagi H: Microcrystals of polydiacetylene derivatives and their linear and nonlinear optical properties. Supramol Sci 1998, 5: 289–295. 10.1016/S0968-5677(98)00021-2View ArticleGoogle Scholar
- Kasai H, Kamatani H, Okada S, Oikawa H, Matsuda H, Nakanishi H: Size-dependent colors and luminescences of organic microcrystals. Jpn J Appl Phys 1996, 35: L221-L223. 10.1143/JJAP.35.L221View ArticleGoogle Scholar
- Oikawa H, Mitsui T, Onodera T, Kasai H, Nakanishi H, Sekiguchi T: Crystal size dependence of fluorescence spectra from perylene nanocrystals evaluated by scanning near-field optical microspectroscopy. Jpn J Appl Phys 2003, 42: L111-L113. 10.1143/JJAP.42.L111View ArticleGoogle Scholar
- Oikawa H: Hybridized organic nanocrystals for optically functional materials. B Chem Soc Jpn 2011, 84: 233–250. 10.1246/bcsj.20100215View ArticleGoogle Scholar
- Onodera T, Oikawa H, Masuhara A, Kasai H, Sekiguchi T, Nakanishi H: Silver-deposited polydiacetylene nanocrystals produced by visible-light-driven photocatalytic reduction. Jpn J Appl Phys 2007, 46: L336-L338. 10.1143/JJAP.46.L336View ArticleGoogle Scholar
- Baba K, Pudavar HE, Roy I, Ohulchanskyy TY, Chen YH, Pandey RK, Prasad PN: New method for delivering a hydrophobic drug for photodynamic therapy using pure nanocrystal form of the drug. Mol Pharmaceut 2007, 4: 289–297. 10.1021/mp060117fView ArticleGoogle Scholar
- Baba K, Kasai H, Masuhara A, Oikawa H, Nakanishi H: Organic solvent-free fluorescence confocal imaging of living cells using pure nanocrystal forms of fluorescent dyes. Jpn J Appl Phys 2009, 48: 117002. 10.1143/JJAP.48.117002View ArticleGoogle Scholar
- Baba K, Tanaka Y, Kubota A, Kasai H, Yokokura S, Nakanishi H, Nishida K: A method for enhancing the ocular penetration of eye drops using nanoparticles of hydrolyzable dye. J Control Release 2011, 153: 278–287. 10.1016/j.jconrel.2011.04.019View ArticleGoogle Scholar
- Kasai H, Murakami T, Ikuta Y, Koseki Y, Baba K, Oikawa H, Nakanishi H, Okada M, Shoji M, Ueda M, Imahori H, Hashida M: Creation of pure nanodrugs and their anticancer properties. Angewe Chem Int Edit 2012, 51: 10315–10318. 10.1002/anie.201204596View ArticleGoogle Scholar
- Baba K, Konta S, Oliveira D, Sugai K, Onodera T, Masuhara A, Kasai H, Oikawa H, Nakanishi H: Perylene and perylene-derivative nano-cocrystals: preparation and physicochemical property. Jpn J Appl Phys 2012, 51: 125201.View ArticleGoogle Scholar
- Fang HH, Yang J, Ding R, Feng J, Chena Q-D, Sun H-B: Top down fabrication of organic nanocrystals by femtosecond laser induced transfer method. Cryst Eng Comm 2012, 14: 4596–4600. 10.1039/c2ce06579gView ArticleGoogle Scholar
- Fang HH, Ding R, Lu SY, Wang L, Feng J, Chen QD, Sun HB: Direct laser interference ablating nanostructures on organic crystals. Opt Lett 2012, 37: 686–688. 10.1364/OL.37.000686View ArticleGoogle Scholar
- Nishi T, Takeichi A, Azuma H, Suzuki N, Hioki T, Motohiro T: Fabrication of palladium nanoparticles by laser ablation in liquid. J Laser Micro Nanoeng 2010, 5: 192–196. 10.2961/jlmn.2010.03.0002View ArticleGoogle Scholar
- Kenth S, Sylvestre JP, Fuhrmann K, Meunier M, Leroux JC: Fabrication of paclitaxel nanocrystals by femtosecond laser ablation and fragmentation. J Pharm Sci 2011, 100: 1022–1030. 10.1002/jps.22335View ArticleGoogle Scholar
- Hobley J, Nakamori T, Kajimoto S, Kasuya M, Hatanaka K, Fukumura H, Nishio S: Formation of 3,4,9,10-perylenetetracarboxylicdianhydride nanoparticles with perylene and polyyne byproducts by 355 nm nanosecond pulsed laser ablation of microcrystal suspensions. J Photoch Photobio A 2007, 189: 105–113. 10.1016/j.jphotochem.2007.01.016View ArticleGoogle Scholar
- Kasai H, Nalwa HS, Oikawa H, Okada S, Matsuda H, Minami N, Kakuta A, Ono K, Mukoh A, Nakanishi H: A novel preparation method of organic microcrystals. Jpn J Appl Phys 1992, 31: L1132-L1134. 10.1143/JJAP.31.L1132View ArticleGoogle Scholar
- Ujiiye-Ishii K, Baba K, Wei Z, Kasai H, Nakanishi H, Okada S, Oikawa H: Mass-production of pigment nanocrystals by the reprecipitation method and their encapsulation. Mol Cryst Liq Cryst 2006, 445: 177–183.View ArticleGoogle Scholar
- Oikawa H, Onodera T, Masuhara A, Kasai H, Nakanishi H: New class materials of organic–inorganic hybridized nanocrystals/nanoparticles, and their assembled micro- and nano-structure toward photonics. Polym Mat Adv Polym Sci 2010, 231: 147–190.View ArticleGoogle Scholar
- Varghese S, Park SK, Casado S, Fischer RC, Resel R, Milian-Medina B, Wannemacher R, Park SY, Gierschner J: Stimulated emission properties of sterically modified distyrylbenzene-based H-aggregate single crystals. J Phys Chem Lett 2013, 4: 1597–1602. 10.1021/jz400659bView ArticleGoogle Scholar
- Lakowicz JR: Principles of Fluorescence Spectroscopy. New York: Springer; 2006.View ArticleGoogle Scholar
- Brouwer AM: Standards for photoluminescence quantum yield measurements in solution (IUPAC Technical Report). Pure Appl Chem 2011, 83: 2213–2228. 10.1351/PAC-REP-10-09-31View ArticleGoogle Scholar
- Baba K, Kasai H, Okada S, Nakanishi H, Oikawa H: Fabrication of diacetylene nanofibers and their dynamic behavior in the course of solid-state polymerization. Mol Cryst Liq Cryst 2006, 445: 161–166.View ArticleGoogle Scholar
- Takahashi S, Miura H, Kasai H, Okada S, Oikawa H, Nakanishi H: Single-crystal-to-single-crystal transformation of diolefin derivatives in nanocrystals. J Am Cheml Soc 2002, 124: 10944–10945. 10.1021/ja026564fView ArticleGoogle Scholar
- Baba K, Kasai H, Okada S, Oikawa H, Nakanishi H: Fabrication of organic nanocrystals using microwave irradiation and their optical properties. Opt Mater 2003, 21: 591–594. 10.1016/S0925-3467(02)00206-9View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.